# ZE41A (ZE41A-T5, 3.5101, M16410) Magnesium

ZE41A magnesium is a magnesium alloy. It is typically furnished in the T5 temper. To achieve this temper, the metal is artificially aged until it meets standard mechanical property requirements. ZE41A is the ASTM designation for this material. 3.5101 is the EN numeric designation. And M16410 is the UNS number.

It has a moderately high density among magnesium alloys. In addition, it has a fairly high base cost and a moderately high thermal conductivity.

The graph bars on the material properties cards below compare ZE41A magnesium to other magnesium alloys (top) and the entire database (bottom).

## Mechanical Properties

Brinell Hardness

63

Compressive (Crushing) Strength

350 *MPa* 50 *x 10 ^{3} psi*

Elastic (Young's, Tensile) Modulus

45 *GPa* 6.6 *x 10 ^{6} psi*

Elongation at Break

3.3 *%*

Fatigue Strength

98 *MPa* 14 *x 10 ^{3} psi*

Fracture Toughness

16 *MPa-m ^{1/2}* 14290

*psi-in*

^{1/2}Poisson's Ratio

0.29

Shear Modulus

18 *GPa* 2.6 *x 10 ^{6} psi*

Shear Strength

150 *MPa* 22 *x 10 ^{3} psi*

Tensile Strength: Ultimate (UTS)

210 *MPa* 30 *x 10 ^{3} psi*

Tensile Strength: Yield (Proof)

140 *MPa* 21 *x 10 ^{3} psi*

## Thermal Properties

Melting Completion (Liquidus)

640 *°C* 1180 *°F*

Melting Onset (Solidus)

540 *°C* 1010 *°F*

Solidification (Pattern Maker's) Shrinkage

1.3 *%*

Specific Heat Capacity

970 *J/kg-K* 0.23 *BTU/lb-°F*

Thermal Conductivity

110 *W/m-K* 63 *BTU/h-ft-°F*

Thermal Expansion

27 *µm/m-K*

## Electrical Properties

Electrical Conductivity: Equal Volume

27 *% IACS*

Electrical Conductivity: Equal Weight (Specific)

130 *% IACS*

## Otherwise Unclassified Properties

Base Metal Price

18 *% relative*

Density

1.9 *g/cm ^{3}* 120

*lb/ft*

^{3}Embodied Carbon

24 *kg CO _{2}/kg material*

Embodied Energy

170 *MJ/kg* 75 *x 10 ^{3} BTU/lb*

Embodied Water

940 *L/kg* 110 *gal/lb*

## Common Calculations

Resilience: Ultimate (Unit Rupture Work)

6.1 *MJ/m ^{3}*

Resilience: Unit (Modulus of Resilience)

220 *kJ/m ^{3}*

Stiffness to Weight: Axial

13 *points*

Stiffness to Weight: Bending

63 *points*

Strength to Weight: Axial

31 *points*

Strength to Weight: Bending

41 *points*

Thermal Diffusivity

59 *m ^{2}/s*

Thermal Shock Resistance

12 *points*

## Alloy Composition

Mg | 91.7 to 95.4 | |

Zn | 3.5 to 5.0 | |

Zr | 0.4 to 1.0 | |

Mn | 0 to 0.15 | |

Cu | 0 to 0.1 | |

Si | 0 to 0.010 | |

Ni | 0 to 0.010 | |

Fe | 0 to 0.010 | |

rare e. | 0.75 to 1.8 | |

res. | 0 to 0.3 |

All values are % weight. Ranges represent what is permitted under applicable standards.

## Followup Questions

## Similar Alloys

## Further Reading

ASTM B80: Standard Specification for Magnesium-Alloy Sand Castings

ASTM B403: Standard Specification for Magnesium-Alloy Investment Castings

Environmental Degradation of Advanced and Traditional Engineering Materials, Lloyd H. Hihara et al., 2014.

Welding and Joining of Magnesium Alloys, Liming Liu ed., 2010

ISO 16220: Magnesium and magnesium alloys - Magnesium alloy ingots and castings